This document specifies a method for determining the flexural properties of rigid and semi-rigid plastics under defined conditions. A preferred test specimen is defined, but parameters are included for alternative specimen sizes for use where appropriate. A range of test speeds is included.
The method is used to investigate the flexural behaviour of the test specimens and to determine the flexural strength, flexural modulus and other aspects of the flexural stress/strain relationship under the conditions defined. It applies to a freely supported beam, loaded at midspan (three-point loading test).
The method is suitable for use with the following range of materials:
— thermoplastic moulding, extrusion and casting materials, including filled and reinforced compounds in addition to unfilled types; rigid thermoplastics sheets;
— thermosetting moulding materials, including filled and reinforced compounds; thermosetting sheets.
In agreement with ISO 10350-1 and ISO 10350-2, this document applies to fibre-reinforced compounds with fibre lengths ≤7,5 mm prior to processing. For long-fibre-reinforced materials (laminates) with fibre lengths >7,5 mm, see ISO 14125.
The method is not normally suitable for use with rigid cellular materials or sandwich structures containing cellular material. In such cases, ISO 1209-1 and/or ISO 1209-2 can be used.
NOTE 1 For certain types of textile-fibre-reinforced plastic, a four-point bending test is used. This is described in ISO 14125.
The method is performed using specimens which can be either moulded to the specified dimensions, machined from the central section of a standard multipurpose test specimen (see ISO 20753) or machined from finished or semi-finished products, such as mouldings, laminates, or extruded or cast sheet.
The method specifies the preferred dimensions for the test specimen. Tests which are carried out on specimens of different dimensions, or on specimens which are prepared under different conditions, can produce results which are not comparable. Other factors, such as the test speed and the conditioning of the specimens, can also influence the results.
NOTE 2 Especially for injection moulded semi-crystalline polymers, the thickness of the oriented skin layer, which is dependent on the moulding conditions, also affects the flexural properties.
The method is not suitable for the determination of design parameters but can be used in materials testing and as a quality control test.
Status: PublishedPublication date: 2019-04
Edition: 6Number of pages: 25
Technical Committee: ISO/TC 61/SC 2 Mechanical behavior
Buy this standard
|std 1 124||PDF + ePub|
|std 2 124||Paper|